Research Article Heat Dissipation of Resonant Absorption in ... › publication › fulltext › Heat-Dissi... › publication › fulltext › Heat-Dissi...by JR Dunklin · 2017 · Cited by 10 — Heat Dissipation of Resonant Absorption in Metal ... The present work eva
Research Article Heat Dissipation of Resonant Absorption in Metal Nanoparticle-Polymer Films Described at Particle Separation Near Resonant Wavelength Jeremy R. Dunklin1 and D. Keith Roper1,2 1
Ralph E. Martin Department of Chemical Engineering, University of Arkansas, Fayetteville, AR 72701, USA Microelectronics-Photonics Graduate Program, University of Arkansas, Fayetteville, AR 72701, USA
Correspondence should be addressed to D. Keith Roper; [email protected]
Received 4 September 2016; Accepted 25 December 2016; Published 26 January 2017 Academic Editor: Ilaria Fratoddi Copyright © 2017 Jeremy R. Dunklin and D. Keith Roper. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Polymer films containing plasmonic nanostructures are of increasing interest for development of responsive energy, sensing, and therapeutic systems. The present work evaluates heat dissipated from power absorbed by resonant gold (Au) nanoparticles (NP) with negligible Rayleigh scattering cross sections randomly dispersed in polydimethylsiloxane (PDMS) films. Finite element analysis (FEA) of heat transport was coordinated with characterization of resonant absorption by Mie theory and coupled dipole approximation (CDA). At AuNP particle separation greater than resonant wavelength, correspondence was observed between measured and CDA-predicted optical absorption and FEA-derived power dissipation. At AuNP particle separation less than resonant wavelength, measured extinction increased relative to predicted values, while FEA-derived power dissipation remained comparable to CDA-predicted power absorption before lagging observed extinguished power at higher AuNP content and resulting particle separation. Effects of isolated particles, for example, scattering, and particle-particle interactions, for example, multiple scattering, aggregation on observed optothermal activity were evaluated. These complementary approaches to distinguish contributions to resonant heat dissipation from isolated particle absorption and interparticle interactions support design and adaptive control of thermoplasmonic materials for a variety of implementations.
1. Introduction Thermal damping of resonant nanoparticles (NPs) dispersed in optically transparent polymer could affect potential implementations in biomedical therapeutics [1, 2], solar cells [3– 6], optical interconnects [7–9], sensing [10–12], and chemical separation . Optical damping by subwavelength Mie scatterers  in the Rayleigh regime  whose scattering cross sections are negligible  is due to absorption . Resonant power absorption of isolated nanoparticles  and colloid suspensions  in homogeneous dielectric environments is describable using Beer-Lambert linearization [19, 20] of Mie theory. Interactions between isolated subwavelength scatterers and their effects on absorption require more extensive characterization, such as dipole approximation [21, 22], finite difference time domain, or T-matrix. Additionally, interference to forward scattering, for example, reflection, refraction,
or diffraction, due to an obstacle,  dielectric interface , applied field [25, 26], or other heterogeneity, may also impact optical extinction [27–29], thermal dynamics , and temperature dispersion [31–33]. Evaluation of heat dissipated from power absorbed in nanocomposites to distinguish contributions from isolated scatterers, interacting scatterers, and heterogeneity is important to advance understanding and guide design of thermally responsive nanocomposite materials. Mie’s solution to Maxwell’s equations elegantly determines scattering and absorption of an electromagnetic plane wave by an isolated, homogenous sphere . The solution, which depends on particle geometry, composition, surrounding dielectric medium, and angle of incidence, allows calculation of efficiencies and cross sections of scattering and absorption as well as intensity distributions. The coupled dipole approximation (CDA) to Maxwell’s
2 equations incorporates Mie particle polarizability and also accounts for interparticle interactions [21, 22]. Multiplying the extinction cross section from homogeneous nanocomposite media containing spherical particles determined via Mie or CDA by the number of particles yields the overall optical response . This is valid when absorbance is linearly proportional to concentration, as in Beer-Lambert law . Beer-Lambert’s law, 𝐴 = 𝜎𝑐𝑙, relates spectral absorbance, A, to AuNP concentration, c, and optical pathlength, 𝑙, using a material- and wavelength-specific absorbance coefficient, 𝜎 [17, 36]. Deviations from Mie and Beer-Lambert Law arise due to particle interactions, for example, multiple scattering, or strongly absorbing media [37, 38]. For nanoparticles in the Rayleigh regime with appreciable absorption cross section, damping of resonant absorption yields a strong photothermal response influenced by incident inten